Jul 14, 2009  T. Coleridge, R. Stoner, and R. Fletcher, Phys. Rev. B 39, 1120 (1989). 'r D. Schoenberg, Magnetic Oscillations in Metals (Cambridge University.
University of Warwick institutional repository: http://go.warwick.ac.uk/wrap This paper is made available online in accordance with publisher policies. Please scroll down to view the document itself. Please refer to the repository record for this item and our policy information available from the repository home page for further information. To see the final version of this paper please visit the publisher’s website. Access to the published version may require a subscription. Author(s): T. E. Whall, N. L. Mattey, A. D. Plews, P. J. Phillips, O. A. Mironov, R. J. Nicholas, and M. J. Kearney Article Title: Effective mass and quantum lifetime in a Si/Si0.87Ge0.13/Si twodimensional hole gas Year of publication: 1994 Link to published version: http://dx.doi.org/ 10.1063/1.111147 Publisher statement: none
Effective mass and quantum twodimensional hole gas
lifetime
in a Si/SJ,&e0.,3/Si
T. E. Whall, N. L. Mattey, A. D. Plews, and P. J. Phillips Department of Physics, University of Warwick, Coventry, CV4 7AL, United Kingdom
0. A. Mironov Institute of Radiophysics and Electronics, Academy of Science of Ukraine, Kharkoy Ukraine
R. J. Nicholas Clarendon Laboratory, Parks Road Oxford University, Oxford, OX1 3PU, United Kingdom
M. J. Kearney
I
GEC Marconi Ltd, Hirst Research Centre, Elstree Way, Borehamwoorl Hertfordshire, WLI6 IRY, United Kingdom
(Received 23 August 1993; accepted for publication 16 November 1993) Measurements of Shubnikov de Haas oscillations in the temperature range 0.32 K have been used to determine an effective mass of 0.23 m. in a Si/Si,,,Ge,,,,/Si twodimensional hole gas. This value is in agreement with theoretical predictions and with that obtained from cyclotron resonance measurements. The ratio of the transport time to the quantum lifetime is found to be 0.8. It is concluded that the 4 K hole mobility of 11 000 cm’ Vl sl at a carrier sheet density of 2.2X1011 cm’ is limitid by interface roughness and shortrange interface charge scattering.
One of the most important consequences of the presence of strain and confinement in SiGe/Si heterostructures is the predicted reduction of the hole effective mass caused by the lifting of the degeneracy of the light and heavy hole bands. For a completely decoupled system, which occurs for high strain and low carrier densities the heavy hole mass is expected to fall to values of approximately 0.2mo.’ Shubnikov de Haas (SdH) and cyclotron resonance measurements24 have recently been used to determine the effective mass of carriers in the Si/Si,,GeJSi twodimensional hole gas (2DHG). For x=0.15 and a carrier sheet density of the order of lXIO1’ cm’ (Refs. 3 and 4) there is agreement that m*==0.4~. This value is considerably larger than the theoretical value for the decoupled band near k=O, probably due to its large nonparabolicity at relatively high carrier densities. Lower mass values of 0.3m, were found in the first report of a ptype modulationdoped Si/SiGe heterostructure by People et al.,2 who studied a structure with x=0.2 and a carrier sheet density of 4X 1011cme2, and in the recent report of cyclotron resonance4 on a quantum well with x=0.37. In the present work we show that effective mass values can be observed as low as 0.23mo, in structures with x=0.13, when careful studies of SdH oscillations are made on low density and high mobility structures. We also demonstrate that the effective mass so determined is independent of magnetic field and temperature, in contrast to the behavior seen at higher carrier densities in silicon inversion layers,5,6 and obtain information on the carrier scattering mechanisms. This has been made possible by the achievement of record hole mobilities in Si/Si, ,Ge,/Si structures.7 The magnetic field dependence of the longitudinal resistance (p,) has been measured in a sample of concentration x=0.13, and 4 K carrier mobility of 11000 cm’ Vl sl. Figure 1 shows pxx plotted against B for a range of temperatures. A carrier sheet density of 2.2~10~’ cm’ is obtained
with that obtained from Hall measurements. From our previous work’ we expect single subband occupancy at this sheet density and the present SdH data are consistent with this view. The oscillatory component of the magnetoresistance has been obtained by removing the background contribution which is quadratic in B and which is believed to be associated with holehole interactions.g Fast Fourier transform techniques have then been used to eliminate any harmonics, leaving a fundamental component which is assumed to be given by”,”
4 3 2
0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 B/Tesla
FIG. 1. Longitudinal resistance pxx plotted vs magnetic field B for a range
from the period of pxx vs l/B in low fields, in agreement of temperatures. @ 1994 American Institute of Physics 357 00036951/94/64(3)/357/3/$6.00 Appl. Phys. Lett. 64 (3), 17 January 1994 Downloaded 14 Jul 2009 to 137.205.202.8. Redistribution subject to AIP license or copyright; see http://apl.aip.org/apl/copyright.jsp
1

2
s
3
5
4 5 6
4
3
2
0
1
Ln ( [/sinh[
)
FJG. 2. ~n(Ap,/p~) plotted vs In(@sinh &j for various magnetic fields.
~=R,V&exp(~)cos( 2%+4)
(1)
for low enough fields, where pa is the resistance at zero B, 7q is the quantum lifetime, ~=2n%TIiiwC, and tic== eB/m *. The prefactor R, is associated with Zeeman splitting” while 1’ is usually set equal to 4.l’ We will assume that R, and V are independent of magnetic field and temperature in which case they are not involved in the following analysis. This procedure is justified below. Figure 2 shows plots of ln(Ap,/po) vs ln(@sinh 0 in the temperature range 0.32 K, for various values of B, where Ap, is the peak value of Using m” as an adjustable parameter, a gradient of APxr unity is obtained in each case, for a field independent vahre of m*=(0.23~0.02)mo. In Fig. 3 Dingle plots of vs l/B with m*=0.23mo give a uniM&+JMsi~ Y91 versal straight line for various temperatures, confirming that the experimentally determined m* is also independent of temperature. Noting that the gradient of the line is rrc~/p where cyis the ratio r/r4 of the transport time r to the quantum lifetime r4 and p is the Hall mobility, we obtain cu=O.S.
..I
0
5
r
0 0 0
1
T=0.35K T=0.50K T=1.65K
2 .c _ .G 0) x 3 2 :: 4 V ~5 f 6 0
l/B
FIG. 3. Dingle temperatures.
358
2
1 (Tl)
plots of In[(Ap,sinh &)/@,&J vs
l/B
for
Appl. Phys. Lett., Vol. 64, No. 3, 17 January 1994
various
This value should be compared with Gold’s predictions” of LY=1 for scattering by interface charge and a=0.67 for shortrange interface roughness scattering. Therefore, it is consistent with our recent work in which we have concluded that both mechanisms are present for comparable mobilities and sheet densities.7 The presence of alloy scattering could also lead to similar values of a, but recent calculations by Emeleus et aL8 and Gold” of screened alloy scattering suggest that it is comparatively small for structures of the present composition and mobility. In carrying out this analysis we have assumed that V and R, are independent of magnetic field and temperature. The good straight lines in Figs. 2 and 3 provide strong evidence that these assumptions are justified. V is commonly assumed to be a constant,r’ but Bocklemann and coworkers13 have derived an expression for V which is a function of a: B, and T. The incorporation of such a term into Eq. (1) can be shown to have a negligible effect because c~is close to unity. Since the spin spIitting factor Rs=cos(rgm*/2mo),11 the behaviors shown in Figs. 2 and 3 suggest that exchange enhancement of the splitting factor g, which could give rise to a temperature and magnetic field dependence of g, is small in the present case.r4 It should be noted, however, that the spin splitting is large in this ptype system, since the dominant resistivity minima at approximately 1.8 T correspond to the occupancy of an odd number of spin split Landau levels (see Fig. 1). The weaker, higher field, minima appearing at low temperatures and at a field of approximately 2.3 T are at an even occupancy, corresponding to the Fermi level lying between the spin up and spin down states of adjacent Landau levels. This implies that the spin splitting g*,xBB>0.5fioC, and thus using our measured mass value of 0.23mo we find that g” >4.3. This is consistent with the conclusions of Fang et al.,‘” and of Glaser et al. I6 who found from optically detected magnetic resonance a g factor of 4.5. Finally, we have also ignored screening effects which lead to a temperature dependent r4 (Refs. 12, 17, and 18) and weaklocalization and holehole interaction effectsI in determining p0 and ,x, on the basis that these corrections are small in the temperature range considered and for the present mobilities. In conclusion, we obtain m * = (0.23 k0.02)mo for x=0.13 independent of temperature and magnetic field, in good agreement with theoretical predictions1g,20which range from 0.2 to 0.25mo, and with a value of 0.26mo obtained from cyclotron resonance measurements on similar structures.‘1 The ratio of the transport time to the quantum lifetime has been found to be 0.8, which suggests that the mobility is limited by both interface charge and shortrange interface roughness scattering, in agreement with our previous work.7 One of the authors (O.A.M.) thanks the UK Science and Engineering Research Council for financial support. ‘J. C Hensel and G. Feher, Phys. Rev. 129, 1041 (1963). “R. People, J. C. Bean, D. V. Lang, A. M. Stormer, K. W. Wccht, R. T. Lynch, and K Baldwin, Appl. Phys. Lett. 45, 1231 (1984). ‘P. J Wang, P. E Fang, B. S. Meyerson, J. Nocera, and B. Parker, Appl. Phys. Lett. 54, 2701 (1989). 4J. P. Cheng, V. P. Kesan, D. A. Grutzmacher, T. 0. Sedgwick, and J. A. Ott, Appl. Phys. Lett. 62, 1522 (1993). Whall et
Downloaded 14 Jul 2009 to 137.205.202.8. Redistribution subject to AIP license or copyright; see http://apl.aip.org/apl/copyright.jsp
a/.
‘I? F. Fang, A. B. Fowler, and A. Hartsein, Phys. Rev. B 16, 4446 (1977). “A. Hartstein and F. E Fang, Phys. Rev. B 18, 5502 (1978). 7T. E. Whall, D. W. Smith, A. D. Plews, R. A. Kubiak, P. J. Phillips, and E. H. C Parker, Semicond. Sci. Technol. 8, 615 (1993). sC. J. Emeleus, T. E. Whall, D. W. Smith, R. A. Kubiak, E. H. C Parker, and M. J. Kearney, J. Appl. Phys. 73, 3852 (1993). ‘A. Houghton, J. R. Senna, and S. C. Ying, Phys. Rev. B 25, 2196 (1982). ‘OP.T. Coleridge, R. Stoner, and R. Fletcher, Phys. Rev. B 39, 1120 (1989). ‘r D. Schoenberg, Magnetic Oscillations in Metals (Cambridge University Press, Cambridge, 1984). “A GoId, Phys. Rev. B 38, 10798 (1988). r3U. Bockelmann, P. Heirgeist, G. Abstreiter, G .Weimann, and W. Sclapp, Surf. Sci. 229, 398 (1990).
Appl. Phys. Let,
Vol. 64, No. 3, 17 January 1994
14A: Isihara and L. Ioriafti, Physica B 113, 42 (1982). “F. E Fang, I? J. Wang, B. S. Meyerson, J. J. Nocera, and K. E. Ismail, Surf. Sci. 263, 175 (1992). 16E. Glaser>J, M. Trombetta, T. A. Kennedy, S. M. Prokes, 0. J. Glembocki, K. L. Wang, and C H. Chern, Phys. Rev. Lett. 65, 1247 (1990). “A Gold and V. T. Dolgopolov, Phys. Rev. B 33, 1076 (1986). “C: J. Emeleus, T. E. Whall, D. W. Smith, N. L. Mattey, R. A. Kubiak, E. H. C. Parker, and M. J Kearney, Phys. Rev. B 47,10 016 (1993). r9S. K. Chun, and K. I,. Wang, IEEE Trans. Electron Devices ED39, 2153 (1992). ‘“U. Ekenberg (private communication). ‘r R. J. Nicholas (unpublished).
Whall et al.
359
Downloaded 14 Jul 2009 to 137.205.202.8. Redistribution subject to AIP license or copyright; see http://apl.aip.org/apl/copyright.jsp